## Higher-order relaxation magnetic phenomena and a

## hierarchy of first-order relaxation variables

### D. Jou

a### and L. Restuccia

ba_{Universitat Aut}_{onoma de Barcelona, Grup de Fis}_{`} _{´ıca Estad´ıstica, Spain,}

b_{University of Messina, Department of Mathematical and Computer Sciences, Physical Sciences and Earth Sciences, Italy}

Aim and motivation

A theory for magnetic relaxation phenomena was de-veloped by G. A. Kluitenberg and the author in the framework of thermodynamics of irreversible pro-cesses with internal variables. It was shown that if n different types of microscopic irreversible phenom-ena give rise to magnetic relaxation, it is possible to describe these microscopic phenomena introducing n macroscopic axial vectorial internal variables in the expression of the entropy. The total specific magne-tization m is split in n+1 parts m(k) (k = 1, ..., n) , i.e. m = m(0) + n X k=1 m(k). (1)

The following set C of independent variables was
as-sumed
C = C
u, _{αβ}, m, m(1), ..., m(n)
, (2)

where u is the specific internal energy and _{αβ} is the
strain tensor. Using the same procedure applied in
[?], by eliminating the internal variables the following
relaxation equation generalizing Snoek equation was
obtained
χ(0)_{BM}B + χ(1)_{BM} dB
dt + ... + χ
(n−1)
BM
dn−1B
dtn−1 +
dnB
dtn =
χ(0)_{M B}M + χ(1)_{M B}dM
dt + ... + χ
(n)
M B
dnM
dtn + χ
(n+1)
M B
dn+1M
dtn+1 , (3)
where χ(m)_{BM} (m = 0, 1, ..., n − 1) and χ(m)_{M B} (m = 0, 1, ..., n +
1) are characteristic constants of the particular
mate-rial.

This magnetic relaxation relation has the same
mathematical structure of the following stress-strain
relation for mechanical distortional phenomena in
isotropic media, derived in 1968 by G. A. K.,
as-suming that n microscopic phenomena give rise to
i-nelastic strains (slip, dislocations, etc.) and the
to-tal strain tensor _{αβ} is split in n+1 parts, (0)_{αβ} and
(k)_{αβ} (k = 1, ..., n) ,
R(τ )
(d)0τ˜αβ + R
(τ )
(d)1
dτ˜_{αβ}
dt + ... + R
(τ )
(d)n−1
dn−1τ˜_{αβ}
dtn−1 +
dnτ˜_{αβ}
dtn =
R()
(d)0˜αβ+ R
()
(d)1
d˜_{αβ}
dt + ... + R
()
(d)n
dn˜_{αβ}
dtn + R
()
(d)n+1
dn+1˜_{αβ}
dtn+1 . (4)
R(τ )
(d)m (m = 0, 1, ..., n − 1) R
()
(d)m (m = 0, 1, ..., n + 1) are

ma-terial constants and τ˜_{αβ} and ˜_{αβ} are the deviators of the
stress tensor and of the strain tensor, respectively.

If n arbitrary microscopic phenomena give rise to the total polarization vector, by introducing n partial po-larization vectors as n macroscopic vectorial internal variables in the expression of the entropy, the follow-ing dielectric relaxation equation was obtained by the author and G. A. K. in the isotropic case

χ(0)_{EP}E + χ(1)_{EP} dE
dt + ... + χ
(n−1)
EP
dn−1E
dtn−1 +
dnE
dtn =
χ(0)_{P E}P + χ(1)_{P E}dP
dt + ... + χ
(n)
P E
dnP
dtn + χ
(n+1)
P E
dn+1P
dtn+1 , (5)
where E and P are the electric strength field and
the polarization vector, respectively, and χ(k)_{EP} (k =
0, 1, ..., n − 1) and χ(k)_{P E}(k = 0, 1, ..., n + 1) are constant
quantities.

The aim of the present work is to relate the n-th or-der relaxation equation (1) (involving time or-derivatives of the magnetic field B up to the n-th order, and time derivatives of the magnetization M up to (n + 1)-th order) to a hierarchy of first-order relaxation equa-tions. In this way we relate the general equation to the microscopic structure of the system. Finally, we obtain the form of the entropy and its consequences on the hierarchy of relaxation equations. We try the pa-per to be as simple and pedagogical as possible, with a

minimum of physical complexity related to the math-ematical structure of the equations.

Description of the model: a dynamical hierarchy

In the model to be considered we focus our
atten-tion on a magnetic system composed of n sets of spins
(i = 1, 2, ..., n), such that there are N(i) magnetic
parti-cles of the kind i, each of them having mass m_{i}, radius
r_{i}, spin S_{i}, and so on. Thus, their inertia, relaxation
time, magnetization and susceptibility will be
differ-ent for each set of particles. These differences will
show up especially in dynamical phenomena. Here,
we will discuss a simple situation in which the time
scales of the several variables M(i), the
magnetiza-tions of the i-th set, are sufficiently separated to be
considered as a hierarchy of equations with minimal
couplings amongst them. We propose the following
hierarchy of dynamical equations

dM(1)
dt +
1
τ_{1} M
(1) _{=} χ1
τ_{1} B + β1 M
(2)_{,}
dM(2)
dt +
1
τ_{2} M
(2) _{=} χ2
τ_{2} B + γ1 M
(1) _{+ β}
2 M(3),
...
dM(i)
dt +
1
τ_{i} M
(i) _{=} χi
τ_{i} B + γ(i−1) M
(i−1) _{+ β}
i M(i+1),
...
dM(n)
dt +
1
τ_{n} M
(n) _{=} χn
τ_{n} B + γ(n−1) M
(n−1)_{.} _{(6)}

We have assumed that τ_{1} > τ_{2} > τ_{3} > > τ_{n}. We will
denote χi

2 χ_{(i−1)} τi ≡ γi. In these equations, χi is the

magnetic susceptibility of particles i, τ_{i} the magnetic
relaxation time, β_{i} a coefficient that couples variables
i and i + 1, and γ_{i} a coefficient coupling variables i
to i − 1. This coupling may be physically realized, for
instance, through the magnetization of the slower of
the couple of the variables i and i − 1, namely i − 1,
which adds to the external applied magnetic field B
acting on M(i). Since M(i−1) is much slower than
M(i), the value of M(i−1) will not appreciably change
during the relaxation of M(i). On the other side, since
M(i+1) is much faster than M(i), M(i+1) will relax in
a very short time and will also keep practically
con-stant in its final relaxed value during the relaxation
on M(i).

Differentiating equation (6)_{1}, using (6)_{2} for the time
derivative of M(2), and using (6)_{1} to express M(2) in
terms of M(1), dM_{dt}(1) and B, one gets

d2M(1)
dt2 + ξ
(11)
M
dM(1)
dt +ξ
(01)
M M
(1) _{= ξ}(11)
B
dB
dt +ξ
(01)
B B + β1 β2 M
(3)_{,}

with the coefficients

ξ_{M}(11) ≡ 1
τ_{1} +
1
τ_{2},
ξ_{M}(01) ≡ 1
τ_{1}τ_{2} − β1γ1,
ξ_{M}(11) ≡ χ1
τ_{1} ,
ξ_{B}(01) ≡ χ1
τ_{1}τ_{2} + β1
χ_{2}
τ_{2} . (7)
We now differentiate equation (7)_{1}, use the
corre-sponding evolution equation of hierarchy (6) for dM_{dt}(3),
and use (6)_{1} and (6)_{2} to express M(2) and M(3) in terms
of M(1), dM_{dt}(1) and B, and we get

d3M(1)
dt3 + ξ
(22)
M
d2M(1)
dt2 + ξ
(12)
M
dM(1)
dt + ξ
(02)
M M
(1) _{=}
ξ_{B}(22) d
2_{B}
dt2 + ξ
(12)
B
dB
dt + ξ
(02)
B B + β1β2β3 M
(4)_{.} _{(8)}

Note that ξ_{M}(ab) is the coefficient multiplying the
a-the derivative of M(1) in the equation corresponding

to the b-th order of approximation, and analogously
for ξ_{B}(ab), but for the a-th derivative of the magnetic
field B. The corresponding coefficients are given by

ξ_{M}(22) ≡ ξ_{M}(11) + 1
τ_{3},
ξ_{M}(12) ≡ ξ_{M}(01) + γ_{2}β_{2} + 1
τ_{1}τ_{3} +
1
τ_{2}τ_{3},
ξ_{M}(02) ≡ γ2β2
τ_{1} +
1
τ_{1}τ_{2}τ_{3},
ξ_{B}(22) ≡ ξ_{B}(11),
ξ_{B}(12) ≡ ξ_{B}(01) + χ1
τ_{1}τ_{3}
ξ_{B}(02) ≡ γ2β2χ1
τ_{1} +
β_{1}β_{2}χ_{3}
τ_{3} +
χ_{1}
τ_{1}τ_{2}τ_{3}. (9)
In principle, one may obtain a series of recurrence
relations for the coefficients corresponding to
higher-order equations. Here, we stop our calculations, which
become increasingly lengthy and cumbersome, as they
already illustrate the basic concept that hierarchy (6)
may be written in the form of higher-order relation
equation of the form we are considering.

### References

[1] L. Restuccia, G.A. Kluitenberg, On generalizations of the Snoek equation for magnetic relaxation phenomena, Atti Accademia Peloritana dei Pericolanti, LXVII (1989), 141-194. [2] L. Restuccia, (2010). On a thermodynamic theory for

mag-netic relaxation phenomena due to n microscopic phenomena described by n internal variables, Journal of Non-Equilibrium Thermodynamics, 35 (4)(2010), 379 - 413.

[3] L. Restuccia, (2014). Generalizations of Snoek equation for anisotropic media with magnetic relaxation, Archive of Applied Mechanics DOI 10.1007/act s00419-014-0881-7, ISSN 0939-1533, 1-25.

[4] S.R. De Groot, P.Mazur, Non-equilibrium Thermodynam-ics (North-Holland Publishing Company, Amsterdam, 1962). [5] G.A. Kluitenberg, Plasticity and Non-equilibrium

Thermo-dynamics, CISM Lecture Notes (Springer, Wien, New York, 1984)

[6] G. Maugin and W. Muschik, Thermodynamics with in-ternal variables, J. Non-Equilib. Thermodyn., vol.19 1994, 217. [7] G. Maugin, The thermodynamics of nonlinear irreversible

be-haviours, World Scientific, Singapore, 1999.

[8] G. Lebon, D. Jou and J. Casas-Vazquez, Understand-ing Non-Equilibrium Thermodynamics, SprUnderstand-inger, Berlin, 2008. [9] D. Jou, J. Casas-Vazquez, G. Lebon, Extended irreversible

thermodynamics, Springer, Berlin, 2010 (fourth edition).

[10] G.A. Kluitenberg, A thermodynamic derivation of the stress-strain relations for Burgers media and related substances, Physica 38 (1968), 513-548.

[11] L.Restuccia and G.A.Kluitenberg, On generalizations of the Debye equation for dielectric relaxation, Physica A 154 (1988), 157-182.

[12] G.A. Kluitenberg, On dielectric and magnetic relaxation phenomena and non-equilibrium thermodynamics, Physica, 68 (1973), 75-92.

[13] G.A. Kluitenberg, On dielectric and magnetic relaxation phenomena and vectorial internal degrees of freedom in ther-modynamics, Physica A 87 (1977), 302-330.

[14] G.A. Kluitenberg, On vectorial internal variables and di-electric and magnetic relaxation phenomena, Physica A 109 (1981), 91-122.

[15] L.Restuccia and G.A.Kluitenberg, Hidden vectorial variables as splitting operators for the polarization vector in the thermodynamic theory of dielectric relaxation, Journal of Non-Equilibrium Thermodynamics, Vol. 15 (1990), 335-346.